#------------------------------------------------------------------------------
#$Date: 2024-05-05 05:50:17 +0300 (Sun, 05 May 2024) $
#$Revision: 291625 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/71/55/7715585.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7715585
loop_
_publ_author_name
'Mączka, Mirosław'
'Sobczak, Szymon'
'Ptak, Maciej'
'Smółka, Szymon'
'Fedoruk, Katarzyna'
'Dybała, Filip'
'Herman, Artur P.'
'Paraguassu, Waldeci'
'Zaręba, Jan K'
'Kudrawiec, Robert'
'Sieradzki, Adam'
'Katrusiak, Andrzej'
_publ_section_title
;
 Revisiting a (001)-oriented layered lead chloride templated by
 1,2,4-triazolium: structural phase transitions, lattice dynamics and
 broadband photoluminescence.
;
_journal_issue                   16
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              6906
_journal_page_last               6919
_journal_paper_doi               10.1039/d4dt00406j
_journal_volume                  53
_journal_year                    2024
_chemical_formula_moiety         'Cl4 Pb, 2(C2 H4 N3)'
_chemical_formula_sum            'C4 H8 Cl4 N6 Pb'
_chemical_formula_weight         489.15
_chemical_name_systematic        Tz2PbCl4
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_atom_sites_solution_hydrogens   mixed
_audit_creation_date             2023-12-15
_audit_creation_method
;
Olex2 1.5
(compiled 2023.08.24 svn.re1ec1418 for OlexSys, GUI svn.r6817)
;
_audit_update_record
;
2024-03-04 deposited with the CCDC.	2024-03-21 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90.093(5)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   21.4424(18)
_cell_length_b                   8.2994(3)
_cell_length_c                   7.4252(4)
_cell_measurement_reflns_used    5584
_cell_measurement_temperature    199.99(10)
_cell_measurement_theta_max      28.5760
_cell_measurement_theta_min      2.5240
_cell_volume                     1321.38(14)
_computing_cell_refinement       'CrysAlisPro 1.171.42.49 (Rigaku OD, 2022)'
_computing_data_collection       'CrysAlisPro 1.171.42.49 (Rigaku OD, 2022)'
_computing_data_reduction        'CrysAlisPro 1.171.42.49 (Rigaku OD, 2022)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2019/2 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_diffrn_ambient_temperature      200.15
_diffrn_detector_area_resol_mean 8.0772
_diffrn_detector_type            Eos
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.902
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Xcalibur, Eos'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0407
_diffrn_reflns_av_unetI/netI     0.0327
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.902
_diffrn_reflns_limit_h_max       26
_diffrn_reflns_limit_h_min       -28
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            14455
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.902
_diffrn_reflns_theta_full        25.000
_diffrn_reflns_theta_max         28.920
_diffrn_reflns_theta_min         2.632
_exptl_absorpt_coefficient_mu    13.556
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.16005
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.42.49 (Rigaku Oxford Diffraction, 2022)
Empirical absorption correction using spherical harmonics,
implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            colourless
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    2.459
_exptl_crystal_description       block
_exptl_crystal_F_000             896
_exptl_crystal_size_max          0.50
_exptl_crystal_size_mid          0.15
_exptl_crystal_size_min          0.12
_refine_diff_density_max         1.632
_refine_diff_density_min         -3.104
_refine_diff_density_rms         0.193
_refine_ls_extinction_coef       0.0112(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2019/2 (Sheldrick 2019)'
_refine_ls_goodness_of_fit_ref   1.155
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     145
_refine_ls_number_reflns         3127
_refine_ls_number_restraints     61
_refine_ls_restrained_S_all      1.152
_refine_ls_R_factor_all          0.0576
_refine_ls_R_factor_gt           0.0419
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0359P)²+5.1929P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0903
_refine_ls_wR_factor_ref         0.0980
_reflns_Friedel_coverage         0.000
_reflns_number_gt                2470
_reflns_number_total             3145
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d4dt00406j2.cif
_cod_data_source_block           triag2pbcl4_03_200_00
_cod_depositor_comments
'Adding full bibliography for 7715584--7715597.cif.'
_cod_database_code               7715585
_shelx_shelxl_version_number     2018/3
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups, All N(H) groups
2. Restrained distances
 N3A-N2A \\sim N3B-N2B
 with sigma of 0.02
 N3B-C2B \\sim N3A-C2A
 with sigma of 0.02
 N2A-C1A \\sim N2B-C1B
 with sigma of 0.02
 N1B-C1B \\sim N1A-C1A
 with sigma of 0.02
 N1B-C2B \\sim N1A-C2A
 with sigma of 0.02
3. Rigid body (RIGU) restrains
 Cl2, Pb1, Cl1, Cl4, Cl3
 with sigma for 1-2 distances of 0.004 and sigma for 1-3 distances of 0.004
 N3B, N2B, C1B, C2B, N1B
 with sigma for 1-2 distances of 0.004 and sigma for 1-3 distances of 0.004
 N2B, C1B, N1B, N3B, C2B
 with sigma for 1-2 distances of 0.004 and sigma for 1-3 distances of 0.004
4.a Aromatic/amide H refined with riding coordinates:
 N1B(H1B), N1A(H1A), C1A(H1AA), C1B(H1BA), C2A(H2AA), C2B(H2BA)
;
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Pb1 Pb 0.25001(2) 0.49423(2) 0.36234(3) 0.03693(16) Uani 1 1 d . . . . .
Cl1 Cl 0.24984(13) 0.7636(2) 0.1371(2) 0.0584(6) Uani 1 1 d . . . . .
Cl2 Cl 0.25006(14) 0.1898(2) 0.5453(3) 0.0629(7) Uani 1 1 d . . . . .
Cl4 Cl 0.38293(13) 0.4877(2) 0.3583(4) 0.0598(6) Uani 1 1 d . . . . .
Cl3 Cl 0.11704(13) 0.4876(2) 0.3581(4) 0.0598(6) Uani 1 1 d . . . . .
N2A N 0.3959(4) 0.3925(8) 0.8521(10) 0.0526(19) Uani 1 1 d D . . . .
N1B N 0.0891(4) 0.6429(8) 0.8291(10) 0.0553(18) Uani 1 1 d D . . . .
H1B H 0.094184 0.748127 0.831885 0.066 Uiso 1 1 calc R U . . .
N1A N 0.4110(4) 0.6413(8) 0.8289(10) 0.057(2) Uani 1 1 d D . . . .
H1A H 0.405762 0.746504 0.831098 0.069 Uiso 1 1 calc R U . . .
N2B N 0.1043(4) 0.3936(8) 0.8522(11) 0.0536(18) Uani 1 1 d D . . . .
C1A C 0.3681(5) 0.5321(10) 0.8693(14) 0.057(2) Uani 1 1 d D . . . .
H1AA H 0.326049 0.551088 0.903513 0.068 Uiso 1 1 calc R U . . .
C1B C 0.1315(5) 0.5324(10) 0.8674(14) 0.059(2) Uani 1 1 d D . . . .
H1BA H 0.173805 0.551120 0.899725 0.070 Uiso 1 1 calc R U . . .
N3A N 0.4559(4) 0.4090(8) 0.8001(13) 0.065(2) Uani 1 1 d D . . . .
N3B N 0.0442(4) 0.4083(8) 0.7998(12) 0.061(2) Uani 1 1 d D . . . .
C2A C 0.4640(4) 0.5635(9) 0.7838(15) 0.062(3) Uani 1 1 d D . . . .
H2AA H 0.501510 0.613953 0.745926 0.075 Uiso 1 1 calc R U . . .
C2B C 0.0368(4) 0.5630(9) 0.7851(14) 0.061(2) Uani 1 1 d D . . . .
H2BA H -0.000931 0.613347 0.747938 0.074 Uiso 1 1 calc R U . . .
H2B H 0.119(4) 0.289(10) 0.863(10) 0.05(2) Uiso 1 1 d . . . . .
H2A H 0.381(4) 0.284(12) 0.865(12) 0.07(3) Uiso 1 1 d . . . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Pb Pb -3.3944 10.1111 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
1 7 -8 0.0869
0 7 8 0.0832
-1 1 10 0.0738
-1 -12 1 0.4117
1 0 -10 0.0824
-2 12 -1 0.1383
-30 1 0 0.0656
30 0 0 0.0459
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Cl1 Pb1 Cl1 82.229(8) . 4_576 ?
Cl1 Pb1 Cl2 86.18(5) . 4_565 ?
Cl1 Pb1 Cl2 171.47(5) . . ?
Cl1 Pb1 Cl2 106.31(5) 4_576 . ?
Cl1 Pb1 Cl4 90.53(7) . . ?
Cl1 Pb1 Cl3 90.49(7) . . ?
Cl2 Pb1 Cl1 168.41(5) 4_565 4_576 ?
Cl2 Pb1 Cl2 85.288(18) 4_565 . ?
Cl2 Pb1 Cl4 88.79(8) 4_565 . ?
Cl2 Pb1 Cl3 88.97(8) 4_565 . ?
Cl4 Pb1 Cl1 91.34(7) . 4_576 ?
Cl4 Pb1 Cl2 89.34(7) . . ?
Cl4 Pb1 Cl3 177.48(6) . . ?
Cl3 Pb1 Cl1 91.09(7) . 4_576 ?
Cl3 Pb1 Cl2 89.31(7) . . ?
Pb1 Cl1 Pb1 171.37(8) . 4_575 ?
Pb1 Cl2 Pb1 151.25(8) 4_566 . ?
C1A N2A N3A 111.9(7) . . ?
C1A N2A H2A 132(6) . . ?
N3A N2A H2A 116(6) . . ?
C1B N1B H1B 126.7 . . ?
C1B N1B C2B 106.5(7) . . ?
C2B N1B H1B 126.7 . . ?
C1A N1A H1A 125.9 . . ?
C1A N1A C2A 108.3(7) . . ?
C2A N1A H1A 125.9 . . ?
C1B N2B N3B 112.0(7) . . ?
C1B N2B H2B 132(5) . . ?
N3B N2B H2B 116(5) . . ?
N2A C1A N1A 105.5(9) . . ?
N2A C1A H1AA 127.3 . . ?
N1A C1A H1AA 127.3 . . ?
N1B C1B H1BA 126.6 . . ?
N2B C1B N1B 106.7(9) . . ?
N2B C1B H1BA 126.6 . . ?
C2A N3A N2A 104.7(7) . . ?
C2B N3B N2B 103.4(7) . . ?
N1A C2A H2AA 125.2 . . ?
N3A C2A N1A 109.7(8) . . ?
N3A C2A H2AA 125.2 . . ?
N1B C2B H2BA 124.3 . . ?
N3B C2B N1B 111.4(8) . . ?
N3B C2B H2BA 124.3 . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Pb1 Cl1 2.7919(16) . ?
Pb1 Cl1 2.8639(16) 4_576 ?
Pb1 Cl2 2.8064(18) 4_565 ?
Pb1 Cl2 2.8684(17) . ?
Pb1 Cl4 2.851(3) . ?
Pb1 Cl3 2.852(3) . ?
N2A C1A 1.310(10) . ?
N2A N3A 1.350(10) . ?
N2A H2A 0.96(10) . ?
N1B H1B 0.8800 . ?
N1B C1B 1.322(11) . ?
N1B C2B 1.344(11) . ?
N1A H1A 0.8800 . ?
N1A C1A 1.326(11) . ?
N1A C2A 1.351(11) . ?
N2B C1B 1.296(10) . ?
N2B N3B 1.351(10) . ?
N2B H2B 0.93(8) . ?
C1A H1AA 0.9500 . ?
C1B H1BA 0.9500 . ?
N3A C2A 1.300(10) . ?
N3B C2B 1.299(10) . ?
C2A H2AA 0.9500 . ?
C2B H2BA 0.9500 . ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
N2A N3A C2A N1A 1.5(10) . . . . ?
N2B N3B C2B N1B -1.1(9) . . . . ?
C1A N2A N3A C2A -0.7(10) . . . . ?
C1A N1A C2A N3A -1.9(11) . . . . ?
C1B N1B C2B N3B 2.0(11) . . . . ?
C1B N2B N3B C2B -0.3(10) . . . . ?
N3A N2A C1A N1A -0.4(11) . . . . ?
N3B N2B C1B N1B 1.5(11) . . . . ?
C2A N1A C1A N2A 1.4(11) . . . . ?
C2B N1B C1B N2B -2.1(11) . . . . ?
